#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/1/51/69/1516911.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1516911
loop_
_publ_author_name
'Jiao Guo'
'Jin Yang'
'Ying-Ying Liu'
'Jian-Fang Ma'
_publ_section_title
;
 Two new polyoxometalate-templated supramolecular compounds constructed by
 a new tridentate ligand
 2,4,6-tris[1-(4-oxidroxypyridinium)-ylmethyl]-mesitylene
;
_journal_name_full
;
Inorganica Chimica Acta
;
_journal_page_first              51
_journal_page_last               58
_journal_volume                  400
_journal_year                    2013
_chemical_formula_moiety         '2(Mo8 O26), 4(C27 H29 N3 O3), 15(H2 O)'
_chemical_formula_sum            'C108 H146 Mo16 N12 O79'
_chemical_formula_weight         4411.17
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 127.481(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   19.9057(8)
_cell_length_b                   11.0481(3)
_cell_length_c                   24.3389(13)
_cell_measurement_reflns_used    4716
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.4
_cell_measurement_theta_min      3.2
_cell_volume                     4247.6(4)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0385
_diffrn_reflns_av_sigmaI/netI    0.0605
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            15534
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.35
_diffrn_reflns_theta_min         3.18
_exptl_absorpt_coefficient_mu    1.227
_exptl_absorpt_correction_T_max  0.832
_exptl_absorpt_correction_T_min  0.782
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlis (Oxford Diffraction, 2006)
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.713
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2152
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.913
_refine_diff_density_min         -0.837
_refine_diff_density_rms         0.126
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     533
_refine_ls_number_reflns         7662
_refine_ls_number_restraints     99
_refine_ls_restrained_S_all      1.059
_refine_ls_R_factor_all          0.0869
_refine_ls_R_factor_gt           0.0547
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0759P)²+5.2574P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1366
_refine_ls_wR_factor_ref         0.1608
_reflns_number_gt                5298
_reflns_number_total             7662
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ICA-2013-400-51-58-1.cif
_cod_data_source_block           compound-1
_cod_original_cell_volume        4247.6(3)
_cod_original_sg_symbol_Hall     '-p 2ybc'
_cod_original_sg_symbol_H-M      'p 21/c'
_cod_database_code               1516911
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
O1 O 0.1923(7) 1.0474(10) 0.9048(6) 0.145(3) Uani 1 1 d U
H1 H 0.2041 0.9832 0.9257 0.218 Uiso 1 1 calc R
O2 O 0.0038(4) 0.6126(6) 0.5549(3) 0.0755(14) Uani 1 1 d U
O3 O 0.8785(3) 0.8912(6) 0.9328(4) 0.085(2) Uani 1 1 d .
H3 H 0.9165 0.8745 0.9734 0.128 Uiso 1 1 calc R
N1 N 0.3398(4) 1.0930(6) 0.8436(4) 0.0640(18) Uani 1 1 d U
N2 N 0.2200(4) 0.7737(8) 0.6092(4) 0.0816(12) Uani 1 1 d U
N3 N 0.6501(3) 0.7978(5) 0.8815(3) 0.0459(14) Uani 1 1 d .
C1 C 0.0743(6) 0.6614(10) 0.5712(5) 0.0878(13) Uani 1 1 d U
C2 C 0.0775(5) 0.7161(10) 0.5247(5) 0.0881(14) Uani 1 1 d U
H2 H 0.0299 0.7159 0.4785 0.106 Uiso 1 1 calc R
C3 C 0.1514(5) 0.7748(10) 0.5438(5) 0.0857(13) Uani 1 1 d U
H3A H 0.1523 0.8143 0.5105 0.103 Uiso 1 1 calc R
C4 C 0.1467(5) 0.6617(10) 0.6385(5) 0.0854(13) Uani 1 1 d U
H4 H 0.1471 0.6248 0.6731 0.103 Uiso 1 1 calc R
C5 C 0.2175(5) 0.7162(10) 0.6544(5) 0.0833(13) Uani 1 1 d U
H5 H 0.2667 0.7122 0.6998 0.100 Uiso 1 1 calc R
C6 C 0.2972(5) 0.8363(10) 0.6263(5) 0.0798(15) Uani 1 1 d U
H6A H 0.2800 0.9105 0.5996 0.096 Uiso 1 1 calc R
H6B H 0.3238 0.7850 0.6122 0.096 Uiso 1 1 calc R
C7 C 0.2701(5) 1.0475(9) 0.6808(6) 0.089(3) Uani 1 1 d .
H7A H 0.2354 1.0133 0.6351 0.134 Uiso 0.50 1 calc PR
H7B H 0.2861 1.1284 0.6786 0.134 Uiso 0.50 1 calc PR
H7C H 0.2390 1.0494 0.6992 0.134 Uiso 0.50 1 calc PR
H7D H 0.2716 1.1141 0.7068 0.134 Uiso 0.50 1 calc PR
H7E H 0.2209 0.9990 0.6633 0.134 Uiso 0.50 1 calc PR
H7F H 0.2679 1.0780 0.6428 0.134 Uiso 0.50 1 calc PR
C8 C 0.2826(6) 1.1768(9) 0.8301(5) 0.082(3) Uani 1 1 d U
H8 H 0.2781 1.2467 0.8068 0.099 Uiso 1 1 calc R
C9 C 0.2327(7) 1.1650(10) 0.8483(6) 0.096(3) Uani 1 1 d U
H9 H 0.1921 1.2232 0.8364 0.115 Uiso 1 1 calc R
C10 C 0.2426(9) 1.0631(12) 0.8855(7) 0.111(3) Uani 1 1 d U
C11 C 0.3025(8) 0.9742(10) 0.9006(6) 0.093(3) Uani 1 1 d U
H11 H 0.3099 0.9046 0.9252 0.111 Uiso 1 1 calc R
C12 C 0.3468(6) 0.9935(9) 0.8788(5) 0.076(2) Uani 1 1 d U
H12 H 0.3860 0.9349 0.8880 0.091 Uiso 1 1 calc R
C13 C 0.3966(5) 1.1157(8) 0.8259(5) 0.072(3) Uani 1 1 d .
H13A H 0.4507 1.1435 0.8668 0.087 Uiso 1 1 calc RD
H13B H 0.3732 1.1796 0.7915 0.087 Uiso 1 1 calc R
C14 C 0.5515(5) 0.9683(8) 0.9147(4) 0.060(2) Uani 1 1 d .
H14A H 0.5714 0.8973 0.9434 0.090 Uiso 1 1 calc R
H14B H 0.5290 1.0246 0.9298 0.090 Uiso 1 1 calc RD
H14C H 0.5977 1.0053 0.9183 0.090 Uiso 1 1 calc R
C15 C 0.5687(4) 0.7479(7) 0.8619(4) 0.0524(19) Uani 1 1 d .
H15A H 0.5737 0.7349 0.9037 0.063 Uiso 1 1 calc R
H15B H 0.5589 0.6699 0.8399 0.063 Uiso 1 1 calc R
C16 C 0.7201(4) 0.7801(7) 0.9459(4) 0.057(2) Uani 1 1 d .
H16 H 0.7153 0.7446 0.9781 0.069 Uiso 1 1 calc R
C17 C 0.7983(5) 0.8119(8) 0.9664(4) 0.065(2) Uani 1 1 d .
H17 H 0.8455 0.7999 1.0120 0.079 Uiso 1 1 calc R
C18 C 0.8076(4) 0.8631(7) 0.9185(5) 0.060(2) Uani 1 1 d .
C19 C 0.7310(5) 0.8829(7) 0.8511(4) 0.059(2) Uani 1 1 d .
H19 H 0.7329 0.9186 0.8174 0.070 Uiso 1 1 calc R
C20 C 0.6562(4) 0.8509(6) 0.8353(4) 0.0485(18) Uani 1 1 d .
H20 H 0.6070 0.8661 0.7910 0.058 Uiso 1 1 calc R
C21 C 0.4418(6) 0.6780(8) 0.7174(5) 0.068(2) Uani 1 1 d .
H21A H 0.4936 0.6387 0.7534 0.101 Uiso 0.50 1 calc PR
H21B H 0.4428 0.6960 0.6793 0.101 Uiso 0.50 1 calc PR
H21C H 0.3949 0.6254 0.7019 0.101 Uiso 0.50 1 calc PR
H21D H 0.3939 0.6680 0.6696 0.101 Uiso 0.50 1 calc PR
H21E H 0.4448 0.6108 0.7438 0.101 Uiso 0.50 1 calc PR
H21F H 0.4927 0.6813 0.7212 0.101 Uiso 0.50 1 calc PR
C22 C 0.3613(4) 0.8665(8) 0.7018(4) 0.053(2) Uani 1 1 d .
C23 C 0.4324(4) 0.7922(7) 0.7444(4) 0.0482(18) Uani 1 1 d .
C24 C 0.4939(4) 0.8273(6) 0.8141(4) 0.0435(17) Uani 1 1 d .
C25 C 0.4832(4) 0.9333(7) 0.8405(4) 0.0519(19) Uani 1 1 d .
C26 C 0.4107(4) 1.0035(6) 0.7977(4) 0.0519(19) Uani 1 1 d .
C27 C 0.3503(4) 0.9697(7) 0.7279(4) 0.056(2) Uani 1 1 d .
Mo1 Mo 0.35881(4) 0.56608(6) 0.86155(3) 0.0457(2) Uani 1 1 d .
Mo2 Mo 0.28582(4) 0.49635(6) 0.94667(4) 0.0520(2) Uani 1 1 d .
Mo3 Mo 0.46828(3) 0.34689(5) 0.99537(3) 0.03635(18) Uani 1 1 d .
Mo4 Mo 0.53839(4) 0.41480(5) 0.91060(3) 0.04373(19) Uani 1 1 d .
O4 O 0.2519(4) 0.6421(5) 0.9362(3) 0.0741(17) Uani 1 1 d .
O5 O 0.2047(3) 0.4079(6) 0.9279(3) 0.0726(17) Uani 1 1 d .
O6 O 0.2785(3) 0.4798(4) 0.8645(2) 0.0533(13) Uani 1 1 d .
O7 O 0.4243(3) 0.5527(4) 0.9796(2) 0.0391(11) Uani 1 1 d .
O8 O 0.3666(3) 0.3272(4) 0.9719(2) 0.0469(12) Uani 1 1 d .
O9 O 0.5086(3) 0.2064(4) 1.0090(3) 0.0490(12) Uani 1 1 d .
O10 O 0.4356(3) 0.3802(4) 0.9041(2) 0.0440(11) Uani 1 1 d .
O11 O 0.5776(3) 0.2710(4) 0.9283(3) 0.0577(14) Uani 1 1 d .
O12 O 0.6391(3) 0.5061(4) 0.9538(3) 0.0493(12) Uani 1 1 d .
O13 O 0.4938(4) 0.4347(5) 0.8258(3) 0.0645(15) Uani 1 1 d .
O14 O 0.4801(3) 0.6003(4) 0.9098(2) 0.0400(11) Uani 1 1 d .
O15 O 0.3280(4) 0.5240(5) 0.7826(3) 0.0703(16) Uani 1 1 d .
O16 O 0.3240(3) 0.7102(5) 0.8512(3) 0.0647(15) Uani 1 1 d .
O4W O 0.886(2) 0.451(3) 0.7923(16) 0.103(9) Uani 0.25 1 d PU
O1W O 0.2389(13) 0.8664(14) 0.9915(12) 0.132(7) Uani 0.50 1 d P
O2W O 0.8798(14) 0.784(3) 0.8268(13) 0.201(12) Uani 0.50 1 d P
O3W O 0.9598(17) 0.556(2) 0.9030(14) 0.174(9) Uani 0.50 1 d PU
O6W O 0.9588(17) 0.643(5) 0.6581(18) 0.29(2) Uani 0.50 1 d P
O5W O 0.1370(18) 0.860(3) 0.7360(17) 0.099(9) Uani 0.25 1 d PU
O7W O 1.0529(15) 0.440(3) 1.012(3) 0.50(4) Uani 0.75 1 d P
O5WA O 0.0858(18) 0.756(3) 0.7269(17) 0.099(9) Uani 0.25 1 d PU
O5WB O 0.118(3) 0.647(5) 0.768(3) 0.171(17) Uani 0.25 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C10 O1 H1 109.5 . .
C18 O3 H3 109.5 . .
C8 N1 C12 117.5(10) . .
C8 N1 C13 120.2(8) . .
C12 N1 C13 122.0(8) . .
C5 N2 C3 118.8(8) . .
C5 N2 C6 123.6(7) . .
C3 N2 C6 117.6(8) . .
C16 N3 C20 119.2(6) . .
C16 N3 C15 118.6(6) . .
C20 N3 C15 122.0(6) . .
C2 C1 O2 121.8(8) . .
C2 C1 C4 117.4(9) . .
O2 C1 C4 120.7(10) . .
C1 C2 C3 121.1(9) . .
C1 C2 H2 119.5 . .
C3 C2 H2 119.5 . .
N2 C3 C2 119.9(10) . .
N2 C3 H3A 120.0 . .
C2 C3 H3A 120.0 . .
C5 C4 C1 119.6(10) . .
C5 C4 H4 120.2 . .
C1 C4 H4 120.2 . .
N2 C5 C4 123.1(9) . .
N2 C5 H5 118.5 . .
C4 C5 H5 118.5 . .
N2 C6 C22 114.0(8) . .
N2 C6 H6A 108.7 . .
C22 C6 H6A 108.7 . .
N2 C6 H6B 108.7 . .
C22 C6 H6B 108.7 . .
H6A C6 H6B 107.6 . .
C27 C7 H7A 109.5 . .
C27 C7 H7B 109.5 . .
H7A C7 H7B 109.5 . .
C27 C7 H7C 109.5 . .
H7A C7 H7C 109.5 . .
H7B C7 H7C 109.5 . .
C27 C7 H7D 109.5 . .
H7A C7 H7D 141.1 . .
H7B C7 H7D 56.3 . .
H7C C7 H7D 56.3 . .
C27 C7 H7E 109.5 . .
H7A C7 H7E 56.3 . .
H7B C7 H7E 141.1 . .
H7C C7 H7E 56.3 . .
H7D C7 H7E 109.5 . .
C27 C7 H7F 109.5 . .
H7A C7 H7F 56.3 . .
H7B C7 H7F 56.3 . .
H7C C7 H7F 141.1 . .
H7D C7 H7F 109.5 . .
H7E C7 H7F 109.5 . .
C9 C8 N1 123.4(11) . .
C9 C8 H8 118.3 . .
N1 C8 H8 118.3 . .
C8 C9 C10 117.7(11) . .
C8 C9 H9 121.2 . .
C10 C9 H9 121.2 . .
O1 C10 C9 119.4(12) . .
O1 C10 C11 120.6(14) . .
C9 C10 C11 119.9(14) . .
C12 C11 C10 117.2(12) . .
C12 C11 H11 121.4 . .
C10 C11 H11 121.4 . .
C11 C12 N1 124.2(10) . .
C11 C12 H12 117.9 . .
N1 C12 H12 117.9 . .
N1 C13 C26 112.4(7) . .
N1 C13 H13A 109.1 . .
C26 C13 H13A 109.1 . .
N1 C13 H13B 109.1 . .
C26 C13 H13B 109.1 . .
H13A C13 H13B 107.8 . .
C25 C14 H14A 109.5 . .
C25 C14 H14B 109.5 . .
H14A C14 H14B 109.5 . .
C25 C14 H14C 109.5 . .
H14A C14 H14C 109.5 . .
H14B C14 H14C 109.5 . .
N3 C15 C24 114.0(6) . .
N3 C15 H15A 108.8 . .
C24 C15 H15A 108.8 . .
N3 C15 H15B 108.8 . .
C24 C15 H15B 108.8 . .
H15A C15 H15B 107.6 . .
N3 C16 C17 122.5(8) . .
N3 C16 H16 118.8 . .
C17 C16 H16 118.8 . .
C16 C17 C18 119.9(7) . .
C16 C17 H17 120.0 . .
C18 C17 H17 120.0 . .
O3 C18 C17 123.8(7) . .
O3 C18 C19 120.8(8) . .
C17 C18 C19 115.4(7) . .
C20 C19 C18 121.0(7) . .
C20 C19 H19 119.5 . .
C18 C19 H19 119.5 . .
N3 C20 C19 121.9(6) . .
N3 C20 H20 119.1 . .
C19 C20 H20 119.1 . .
C23 C21 H21A 109.5 . .
C23 C21 H21B 109.5 . .
H21A C21 H21B 109.5 . .
C23 C21 H21C 109.5 . .
H21A C21 H21C 109.5 . .
H21B C21 H21C 109.5 . .
C23 C21 H21D 109.5 . .
H21A C21 H21D 141.1 . .
H21B C21 H21D 56.3 . .
H21C C21 H21D 56.3 . .
C23 C21 H21E 109.5 . .
H21A C21 H21E 56.3 . .
H21B C21 H21E 141.1 . .
H21C C21 H21E 56.3 . .
H21D C21 H21E 109.5 . .
C23 C21 H21F 109.5 . .
H21A C21 H21F 56.3 . .
H21B C21 H21F 56.3 . .
H21C C21 H21F 141.1 . .
H21D C21 H21F 109.5 . .
H21E C21 H21F 109.5 . .
C27 C22 C23 120.8(7) . .
C27 C22 C6 119.3(8) . .
C23 C22 C6 119.8(8) . .
C22 C23 C24 118.2(7) . .
C22 C23 C21 120.8(7) . .
C24 C23 C21 120.9(7) . .
C25 C24 C23 120.9(6) . .
C25 C24 C15 119.1(7) . .
C23 C24 C15 119.9(7) . .
C26 C25 C24 119.6(7) . .
C26 C25 C14 121.6(7) . .
C24 C25 C14 118.8(7) . .
C25 C26 C27 119.4(7) . .
C25 C26 C13 120.4(7) . .
C27 C26 C13 120.2(7) . .
C22 C27 C26 120.9(7) . .
C22 C27 C7 119.8(8) . .
C26 C27 C7 119.2(8) . .
O15 Mo1 O16 104.9(3) . .
O15 Mo1 O6 99.9(3) . .
O16 Mo1 O6 101.6(3) . .
O15 Mo1 O14 101.3(3) . .
O16 Mo1 O14 98.6(2) . .
O6 Mo1 O14 145.71(19) . .
O15 Mo1 O7 158.4(2) . .
O16 Mo1 O7 96.6(2) . .
O6 Mo1 O7 76.94(18) . .
O14 Mo1 O7 73.42(17) . .
O15 Mo1 O10 87.1(2) . .
O16 Mo1 O10 165.8(2) . .
O6 Mo1 O10 83.28(19) . .
O14 Mo1 O10 71.26(17) . .
O7 Mo1 O10 71.34(16) . .
O15 Mo1 Mo3 136.4(2) . 3_667
O16 Mo1 Mo3 87.21(18) . 3_667
O6 Mo1 Mo3 118.75(15) . 3_667
O14 Mo1 Mo3 35.14(13) . 3_667
O7 Mo1 Mo3 41.81(11) . 3_667
O10 Mo1 Mo3 78.85(10) . 3_667
O5 Mo2 O4 106.2(3) . .
O5 Mo2 O12 102.4(3) . 3_667
O4 Mo2 O12 97.8(3) . 3_667
O5 Mo2 O6 102.0(3) . .
O4 Mo2 O6 99.3(3) . .
O12 Mo2 O6 144.8(2) 3_667 .
O5 Mo2 O8 90.0(2) . .
O4 Mo2 O8 163.7(2) . .
O12 Mo2 O8 76.69(18) 3_667 .
O6 Mo2 O8 78.35(19) . .
O5 Mo2 O7 159.6(2) . .
O4 Mo2 O7 94.2(2) . .
O12 Mo2 O7 74.49(18) 3_667 .
O6 Mo2 O7 73.79(17) . .
O8 Mo2 O7 69.59(16) . .
O9 Mo3 O8 105.5(2) . .
O9 Mo3 O10 100.8(2) . .
O8 Mo3 O10 97.8(2) . .
O9 Mo3 O14 101.4(2) . 3_667
O8 Mo3 O14 95.4(2) . 3_667
O10 Mo3 O14 150.02(19) . 3_667
O9 Mo3 O7 98.5(2) . 3_667
O8 Mo3 O7 155.9(2) . 3_667
O10 Mo3 O7 78.94(18) . 3_667
O14 Mo3 O7 78.09(17) 3_667 3_667
O9 Mo3 O7 174.4(2) . .
O8 Mo3 O7 80.06(19) . .
O10 Mo3 O7 78.42(18) . .
O14 Mo3 O7 77.50(17) 3_667 .
O7 Mo3 O7 75.91(18) 3_667 .
O9 Mo3 Mo4 90.00(18) . .
O8 Mo3 Mo4 133.57(16) . .
O10 Mo3 Mo4 35.85(14) . .
O14 Mo3 Mo4 124.57(13) 3_667 .
O7 Mo3 Mo4 46.50(12) 3_667 .
O7 Mo3 Mo4 86.22(11) . .
O9 Mo3 Mo1 89.70(16) . 3_667
O8 Mo3 Mo1 130.88(16) . 3_667
O10 Mo3 Mo1 125.36(13) . 3_667
O14 Mo3 Mo1 35.47(13) 3_667 3_667
O7 Mo3 Mo1 46.43(11) 3_667 3_667
O7 Mo3 Mo1 86.29(10) . 3_667
Mo4 Mo3 Mo1 91.65(2) . 3_667
O13 Mo4 O11 104.4(3) . .
O13 Mo4 O12 101.6(2) . .
O11 Mo4 O12 100.9(2) . .
O13 Mo4 O10 100.2(2) . .
O11 Mo4 O10 97.5(2) . .
O12 Mo4 O10 146.8(2) . .
O13 Mo4 O7 160.9(2) . 3_667
O11 Mo4 O7 94.4(2) . 3_667
O12 Mo4 O7 77.83(19) . 3_667
O10 Mo4 O7 73.45(17) . 3_667
O13 Mo4 O14 89.2(2) . .
O11 Mo4 O14 164.2(2) . .
O12 Mo4 O14 83.69(18) . .
O10 Mo4 O14 71.85(17) . .
O7 Mo4 O14 71.68(15) 3_667 .
O13 Mo4 Mo3 134.8(2) . .
O11 Mo4 Mo3 86.01(18) . .
O12 Mo4 Mo3 119.75(16) . .
O10 Mo4 Mo3 34.65(13) . .
O7 Mo4 Mo3 41.92(11) 3_667 .
O14 Mo4 Mo3 78.67(11) . .
Mo1 O6 Mo2 117.3(2) . .
Mo3 O7 Mo4 91.59(15) 3_667 3_667
Mo3 O7 Mo1 91.76(17) 3_667 .
Mo4 O7 Mo1 162.9(2) 3_667 .
Mo3 O7 Mo3 104.09(18) 3_667 .
Mo4 O7 Mo3 97.66(16) 3_667 .
Mo1 O7 Mo3 97.74(16) . .
Mo3 O7 Mo2 163.6(2) 3_667 .
Mo4 O7 Mo2 85.61(15) 3_667 .
Mo1 O7 Mo2 86.47(14) . .
Mo3 O7 Mo2 92.32(14) . .
Mo3 O8 Mo2 118.0(2) . .
Mo3 O10 Mo4 109.5(2) . .
Mo3 O10 Mo1 110.0(2) . .
Mo4 O10 Mo1 103.01(19) . .
Mo4 O12 Mo2 116.2(2) . 3_667
Mo3 O14 Mo1 109.4(2) 3_667 .
Mo3 O14 Mo4 110.33(19) 3_667 .
Mo1 O14 Mo4 104.88(18) . .
O4W O5W O5WA 128(3) 2_656 .
O5WB O5WA O5W 125(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 C10 1.351(17) .
O1 H1 0.8200 .
O2 C1 1.320(11) .
O3 C18 1.270(9) .
O3 H3 0.8200 .
N1 C8 1.344(11) .
N1 C12 1.347(12) .
N1 C13 1.457(12) .
N2 C5 1.296(12) .
N2 C3 1.325(11) .
N2 C6 1.495(11) .
N3 C16 1.334(9) .
N3 C20 1.338(9) .
N3 C15 1.487(8) .
C1 C2 1.318(14) .
C1 C4 1.374(12) .
C2 C3 1.404(13) .
C2 H2 0.9300 .
C3 H3A 0.9300 .
C4 C5 1.356(13) .
C4 H4 0.9300 .
C5 H5 0.9300 .
C6 C22 1.504(11) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
C7 C27 1.541(11) .
C7 H7A 0.9600 .
C7 H7B 0.9600 .
C7 H7C 0.9600 .
C7 H7D 0.9600 .
C7 H7E 0.9600 .
C7 H7F 0.9600 .
C8 C9 1.317(16) .
C8 H8 0.9300 .
C9 C10 1.382(18) .
C9 H9 0.9300 .
C10 C11 1.410(16) .
C11 C12 1.294(14) .
C11 H11 0.9300 .
C12 H12 0.9300 .
C13 C26 1.524(12) .
C13 H13A 0.9700 .
C13 H13B 0.9700 .
C14 C25 1.507(11) .
C14 H14A 0.9600 .
C14 H14B 0.9600 .
C14 H14C 0.9600 .
C15 C24 1.494(10) .
C15 H15A 0.9700 .
C15 H15B 0.9700 .
C16 C17 1.360(11) .
C16 H16 0.9300 .
C17 C18 1.406(12) .
C17 H17 0.9300 .
C18 C19 1.421(11) .
C19 C20 1.340(10) .
C19 H19 0.9300 .
C20 H20 0.9300 .
C21 C23 1.486(11) .
C21 H21A 0.9600 .
C21 H21B 0.9600 .
C21 H21C 0.9600 .
C21 H21D 0.9600 .
C21 H21E 0.9600 .
C21 H21F 0.9600 .
C22 C27 1.387(12) .
C22 C23 1.403(11) .
C23 C24 1.414(10) .
C24 C25 1.414(11) .
C25 C26 1.393(10) .
C26 C27 1.407(11) .
Mo1 O15 1.688(5) .
Mo1 O16 1.692(5) .
Mo1 O6 1.899(5) .
Mo1 O14 1.975(4) .
Mo1 O7 2.328(4) .
Mo1 O10 2.387(5) .
Mo1 Mo3 3.2111(8) 3_667
Mo2 O5 1.694(6) .
Mo2 O4 1.704(6) .
Mo2 O12 1.922(5) 3_667
Mo2 O6 1.925(5) .
Mo2 O8 2.292(5) .
Mo2 O7 2.438(4) .
Mo3 O9 1.686(5) .
Mo3 O8 1.751(5) .
Mo3 O10 1.933(5) .
Mo3 O14 1.960(4) 3_667
Mo3 O7 2.142(4) 3_667
Mo3 O7 2.382(4) .
Mo3 Mo4 3.2049(9) .
Mo3 Mo1 3.2111(8) 3_667
Mo4 O13 1.692(6) .
Mo4 O11 1.705(5) .
Mo4 O12 1.891(5) .
Mo4 O10 1.991(5) .
Mo4 O7 2.326(4) 3_667
Mo4 O14 2.349(5) .
O7 Mo3 2.142(4) 3_667
O7 Mo4 2.326(4) 3_667
O12 Mo2 1.922(5) 3_667
O14 Mo3 1.960(4) 3_667
O4W O5W 1.15(4) 2_646
O5W O4W 1.15(4) 2_656
O5W O5WA 1.46(4) .
O5WA O5WB 1.44(5) .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O1 H1 O1W 0.82 1.83 2.63(2) 164.8 .
C21 H21E O13 0.96 2.52 3.455(11) 164.5 .
C15 H15A O14 0.97 2.46 3.103(8) 123.7 .
O3 H3 O2 0.82 1.67 2.456(9) 160.7 4_676
C12 H12 O9 0.93 2.59 3.324(11) 135.9 3_667
C13 H13A O11 0.97 2.45 3.348(10) 153.8 1_565
C15 H15A O8 0.97 2.58 3.517(10) 161.5 3_667
C16 H16 O5 0.93 2.49 3.224(10) 136.4 3_667
C19 H19 O15 0.93 2.27 3.122(10) 151.7 2_656
C20 H20 O13 0.93 2.40 3.302(9) 164.6 2_656
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O2 C1 C2 C3 175.6(10) . .
C4 C1 C2 C3 -1.4(19) . .
C5 N2 C3 C2 1.2(17) . .
C6 N2 C3 C2 179.3(10) . .
C1 C2 C3 N2 1.2(18) . .
C2 C1 C4 C5 -0.6(18) . .
O2 C1 C4 C5 -177.6(10) . .
C3 N2 C5 C4 -3.3(18) . .
C6 N2 C5 C4 178.7(10) . .
C1 C4 C5 N2 3.1(18) . .
C5 N2 C6 C22 -20.9(15) . .
C3 N2 C6 C22 161.1(10) . .
C12 N1 C8 C9 -1.5(14) . .
C13 N1 C8 C9 -176.0(9) . .
N1 C8 C9 C10 2.7(16) . .
C8 C9 C10 O1 -179.7(11) . .
C8 C9 C10 C11 -2.3(17) . .
O1 C10 C11 C12 178.0(12) . .
C9 C10 C11 C12 0.6(18) . .
C10 C11 C12 N1 0.8(17) . .
C8 N1 C12 C11 -0.4(15) . .
C13 N1 C12 C11 174.1(10) . .
C8 N1 C13 C26 -140.8(8) . .
C12 N1 C13 C26 44.8(11) . .
C16 N3 C15 C24 143.0(7) . .
C20 N3 C15 C24 -42.5(10) . .
C20 N3 C16 C17 -1.3(13) . .
C15 N3 C16 C17 173.4(8) . .
N3 C16 C17 C18 -1.5(14) . .
C16 C17 C18 O3 -177.3(9) . .
C16 C17 C18 C19 2.9(13) . .
O3 C18 C19 C20 178.5(8) . .
C17 C18 C19 C20 -1.7(13) . .
C16 N3 C20 C19 2.5(12) . .
C15 N3 C20 C19 -172.0(7) . .
C18 C19 C20 N3 -0.9(13) . .
N2 C6 C22 C27 -81.7(11) . .
N2 C6 C22 C23 99.9(10) . .
C27 C22 C23 C24 -2.1(11) . .
C6 C22 C23 C24 176.3(7) . .
C27 C22 C23 C21 176.5(7) . .
C6 C22 C23 C21 -5.2(11) . .
C22 C23 C24 C25 1.3(10) . .
C21 C23 C24 C25 -177.3(7) . .
C22 C23 C24 C15 177.4(6) . .
C21 C23 C24 C15 -1.2(10) . .
N3 C15 C24 C25 -74.4(9) . .
N3 C15 C24 C23 109.4(8) . .
C23 C24 C25 C26 0.7(11) . .
C15 C24 C25 C26 -175.5(7) . .
C23 C24 C25 C14 -178.6(7) . .
C15 C24 C25 C14 5.2(10) . .
C24 C25 C26 C27 -1.9(11) . .
C14 C25 C26 C27 177.4(7) . .
C24 C25 C26 C13 178.0(7) . .
C14 C25 C26 C13 -2.8(12) . .
N1 C13 C26 C25 -99.1(9) . .
N1 C13 C26 C27 80.7(10) . .
C23 C22 C27 C26 0.9(11) . .
C6 C22 C27 C26 -177.4(7) . .
C23 C22 C27 C7 -177.9(7) . .
C6 C22 C27 C7 3.8(11) . .
C25 C26 C27 C22 1.1(12) . .
C13 C26 C27 C22 -178.7(8) . .
C25 C26 C27 C7 179.9(8) . .
C13 C26 C27 C7 0.1(12) . .
O9 Mo3 Mo4 O13 105.8(3) . .
O8 Mo3 Mo4 O13 -5.9(3) . .
O10 Mo3 Mo4 O13 -3.0(3) . .
O14 Mo3 Mo4 O13 -150.4(3) 3_667 .
O7 Mo3 Mo4 O13 -152.5(3) 3_667 .
O7 Mo3 Mo4 O13 -78.4(3) . .
Mo1 Mo3 Mo4 O13 -164.5(3) 3_667 .
O9 Mo3 Mo4 O11 -0.7(2) . .
O8 Mo3 Mo4 O11 -112.4(3) . .
O10 Mo3 Mo4 O11 -109.4(3) . .
O14 Mo3 Mo4 O11 103.2(2) 3_667 .
O7 Mo3 Mo4 O11 101.1(2) 3_667 .
O7 Mo3 Mo4 O11 175.2(2) . .
Mo1 Mo3 Mo4 O11 89.02(18) 3_667 .
O9 Mo3 Mo4 O12 -101.0(2) . .
O8 Mo3 Mo4 O12 147.3(3) . .
O10 Mo3 Mo4 O12 150.3(3) . .
O14 Mo3 Mo4 O12 2.9(2) 3_667 .
O7 Mo3 Mo4 O12 0.8(2) 3_667 .
O7 Mo3 Mo4 O12 74.90(19) . .
Mo1 Mo3 Mo4 O12 -11.27(17) 3_667 .
O9 Mo3 Mo4 O10 108.7(3) . .
O8 Mo3 Mo4 O10 -3.0(3) . .
O14 Mo3 Mo4 O10 -147.4(3) 3_667 .
O7 Mo3 Mo4 O10 -149.5(3) 3_667 .
O7 Mo3 Mo4 O10 -75.4(3) . .
Mo1 Mo3 Mo4 O10 -161.6(2) 3_667 .
O9 Mo3 Mo4 O7 -101.7(2) . 3_667
O8 Mo3 Mo4 O7 146.6(3) . 3_667
O10 Mo3 Mo4 O7 149.5(3) . 3_667
O14 Mo3 Mo4 O7 2.1(2) 3_667 3_667
O7 Mo3 Mo4 O7 74.1(2) . 3_667
Mo1 Mo3 Mo4 O7 -12.05(16) 3_667 3_667
O9 Mo3 Mo4 O14 -176.87(19) . .
O8 Mo3 Mo4 O14 71.4(2) . .
O10 Mo3 Mo4 O14 74.4(3) . .
O14 Mo3 Mo4 O14 -73.0(2) 3_667 .
O7 Mo3 Mo4 O14 -75.13(19) 3_667 .
O7 Mo3 Mo4 O14 -1.01(14) . .
Mo1 Mo3 Mo4 O14 -87.17(10) 3_667 .
O15 Mo1 O6 Mo2 179.8(3) . .
O16 Mo1 O6 Mo2 -72.6(3) . .
O14 Mo1 O6 Mo2 52.3(5) . .
O7 Mo1 O6 Mo2 21.6(2) . .
O10 Mo1 O6 Mo2 94.0(3) . .
Mo3 Mo1 O6 Mo2 20.6(3) 3_667 .
O5 Mo2 O6 Mo1 179.7(3) . .
O4 Mo2 O6 Mo1 70.8(3) . .
O12 Mo2 O6 Mo1 -47.3(5) 3_667 .
O8 Mo2 O6 Mo1 -92.8(3) . .
O7 Mo2 O6 Mo1 -20.9(2) . .
O15 Mo1 O7 Mo3 97.3(6) . 3_667
O16 Mo1 O7 Mo3 -78.3(2) . 3_667
O6 Mo1 O7 Mo3 -178.7(2) . 3_667
O14 Mo1 O7 Mo3 18.76(17) . 3_667
O10 Mo1 O7 Mo3 94.09(17) . 3_667
O15 Mo1 O7 Mo4 -161.5(7) . 3_667
O16 Mo1 O7 Mo4 22.9(7) . 3_667
O6 Mo1 O7 Mo4 -77.5(7) . 3_667
O14 Mo1 O7 Mo4 120.0(7) . 3_667
O10 Mo1 O7 Mo4 -164.7(7) . 3_667
Mo3 Mo1 O7 Mo4 101.2(7) 3_667 3_667
O15 Mo1 O7 Mo3 -7.2(7) . .
O16 Mo1 O7 Mo3 177.2(2) . .
O6 Mo1 O7 Mo3 76.8(2) . .
O14 Mo1 O7 Mo3 -85.71(18) . .
O10 Mo1 O7 Mo3 -10.39(15) . .
Mo3 Mo1 O7 Mo3 -104.5(2) 3_667 .
O15 Mo1 O7 Mo2 -99.0(6) . .
O16 Mo1 O7 Mo2 85.4(2) . .
O6 Mo1 O7 Mo2 -15.03(18) . .
O14 Mo1 O7 Mo2 -177.58(18) . .
O10 Mo1 O7 Mo2 -102.25(16) . .
Mo3 Mo1 O7 Mo2 163.7(2) 3_667 .
O8 Mo3 O7 Mo3 178.5(2) . 3_667
O10 Mo3 O7 Mo3 -81.3(2) . 3_667
O14 Mo3 O7 Mo3 80.66(19) 3_667 3_667
O7 Mo3 O7 Mo3 0.0 3_667 3_667
Mo4 Mo3 O7 Mo3 -46.00(14) . 3_667
Mo1 Mo3 O7 Mo3 45.91(14) 3_667 3_667
O8 Mo3 O7 Mo4 84.9(2) . 3_667
O10 Mo3 O7 Mo4 -174.93(19) . 3_667
O14 Mo3 O7 Mo4 -12.92(16) 3_667 3_667
O7 Mo3 O7 Mo4 -93.59(18) 3_667 3_667
Mo4 Mo3 O7 Mo4 -139.58(13) . 3_667
Mo1 Mo3 O7 Mo4 -47.68(12) 3_667 3_667
O8 Mo3 O7 Mo1 -87.7(2) . .
O10 Mo3 O7 Mo1 12.44(17) . .
O14 Mo3 O7 Mo1 174.4(2) 3_667 .
O7 Mo3 O7 Mo1 93.8(2) 3_667 .
Mo4 Mo3 O7 Mo1 47.79(12) . .
Mo1 Mo3 O7 Mo1 139.69(13) 3_667 .
O8 Mo3 O7 Mo2 -0.94(18) . .
O10 Mo3 O7 Mo2 99.18(17) . .
O14 Mo3 O7 Mo2 -98.81(17) 3_667 .
O7 Mo3 O7 Mo2 -179.5(2) 3_667 .
Mo4 Mo3 O7 Mo2 134.54(11) . .
Mo1 Mo3 O7 Mo2 -133.56(11) 3_667 .
O5 Mo2 O7 Mo3 180.0(8) . 3_667
O4 Mo2 O7 Mo3 0.8(8) . 3_667
O12 Mo2 O7 Mo3 -96.1(8) 3_667 3_667
O6 Mo2 O7 Mo3 99.3(8) . 3_667
O8 Mo2 O7 Mo3 -177.4(8) . 3_667
O5 Mo2 O7 Mo4 -99.3(7) . 3_667
O4 Mo2 O7 Mo4 81.4(2) . 3_667
O12 Mo2 O7 Mo4 -15.48(16) 3_667 3_667
O6 Mo2 O7 Mo4 179.92(19) . 3_667
O8 Mo2 O7 Mo4 -96.75(17) . 3_667
O5 Mo2 O7 Mo1 95.8(7) . .
O4 Mo2 O7 Mo1 -83.4(2) . .
O12 Mo2 O7 Mo1 179.64(19) 3_667 .
O6 Mo2 O7 Mo1 15.04(17) . .
O8 Mo2 O7 Mo1 98.37(17) . .
O5 Mo2 O7 Mo3 -1.8(7) . .
O4 Mo2 O7 Mo3 179.0(2) . .
O12 Mo2 O7 Mo3 82.02(18) 3_667 .
O6 Mo2 O7 Mo3 -82.57(19) . .
O8 Mo2 O7 Mo3 0.75(14) . .
O9 Mo3 O8 Mo2 -179.2(3) . .
O10 Mo3 O8 Mo2 -75.6(3) . .
O14 Mo3 O8 Mo2 77.4(3) 3_667 .
O7 Mo3 O8 Mo2 4.6(6) 3_667 .
O7 Mo3 O8 Mo2 1.1(2) . .
Mo4 Mo3 O8 Mo2 -73.8(3) . .
Mo1 Mo3 O8 Mo2 77.3(3) 3_667 .
O5 Mo2 O8 Mo3 177.9(3) . .
O4 Mo2 O8 Mo3 -7.6(10) . .
O12 Mo2 O8 Mo3 -79.3(3) 3_667 .
O6 Mo2 O8 Mo3 75.7(3) . .
O7 Mo2 O8 Mo3 -1.2(2) . .
O9 Mo3 O10 Mo4 -74.6(3) . .
O8 Mo3 O10 Mo4 177.8(2) . .
O14 Mo3 O10 Mo4 62.6(5) 3_667 .
O7 Mo3 O10 Mo4 22.0(2) 3_667 .
O7 Mo3 O10 Mo4 99.7(2) . .
Mo1 Mo3 O10 Mo4 22.8(3) 3_667 .
O9 Mo3 O10 Mo1 172.9(2) . .
O8 Mo3 O10 Mo1 65.3(2) . .
O14 Mo3 O10 Mo1 -49.9(5) 3_667 .
O7 Mo3 O10 Mo1 -90.5(2) 3_667 .
O7 Mo3 O10 Mo1 -12.79(17) . .
Mo4 Mo3 O10 Mo1 -112.5(3) . .
Mo1 Mo3 O10 Mo1 -89.70(19) 3_667 .
O13 Mo4 O10 Mo3 177.9(2) . .
O11 Mo4 O10 Mo3 71.6(3) . .
O12 Mo4 O10 Mo3 -51.8(5) . .
O7 Mo4 O10 Mo3 -20.70(19) 3_667 .
O14 Mo4 O10 Mo3 -96.4(2) . .
O13 Mo4 O10 Mo1 -65.2(2) . .
O11 Mo4 O10 Mo1 -171.4(2) . .
O12 Mo4 O10 Mo1 65.1(4) . .
O7 Mo4 O10 Mo1 96.26(18) 3_667 .
O14 Mo4 O10 Mo1 20.60(15) . .
Mo3 Mo4 O10 Mo1 117.0(3) . .
O15 Mo1 O10 Mo3 -165.3(3) . .
O16 Mo1 O10 Mo3 46.2(11) . .
O6 Mo1 O10 Mo3 -64.9(2) . .
O14 Mo1 O10 Mo3 91.8(2) . .
O7 Mo1 O10 Mo3 13.55(18) . .
Mo3 Mo1 O10 Mo3 56.22(17) 3_667 .
O15 Mo1 O10 Mo4 78.1(3) . .
O16 Mo1 O10 Mo4 -70.4(10) . .
O6 Mo1 O10 Mo4 178.5(2) . .
O14 Mo1 O10 Mo4 -24.83(19) . .
O7 Mo1 O10 Mo4 -103.1(2) . .
Mo3 Mo1 O10 Mo4 -60.42(14) 3_667 .
O13 Mo4 O12 Mo2 -177.4(3) . 3_667
O11 Mo4 O12 Mo2 -70.0(3) . 3_667
O10 Mo4 O12 Mo2 52.6(5) . 3_667
O7 Mo4 O12 Mo2 22.1(2) 3_667 3_667
O14 Mo4 O12 Mo2 94.7(3) . 3_667
Mo3 Mo4 O12 Mo2 21.6(3) . 3_667
O15 Mo1 O14 Mo3 179.7(3) . 3_667
O16 Mo1 O14 Mo3 72.5(3) . 3_667
O6 Mo1 O14 Mo3 -53.1(5) . 3_667
O7 Mo1 O14 Mo3 -21.87(19) . 3_667
O10 Mo1 O14 Mo3 -97.3(2) . 3_667
O15 Mo1 O14 Mo4 -62.0(3) . .
O16 Mo1 O14 Mo4 -169.2(2) . .
O6 Mo1 O14 Mo4 65.2(4) . .
O7 Mo1 O14 Mo4 96.46(19) . .
O10 Mo1 O14 Mo4 21.03(16) . .
Mo3 Mo1 O14 Mo4 118.3(3) 3_667 .
O13 Mo4 O14 Mo3 -166.7(3) . 3_667
O11 Mo4 O14 Mo3 43.0(8) . 3_667
O12 Mo4 O14 Mo3 -65.0(2) . 3_667
O10 Mo4 O14 Mo3 92.3(2) . 3_667
O7 Mo4 O14 Mo3 14.27(18) 3_667 3_667
Mo3 Mo4 O14 Mo3 57.12(17) . 3_667
O13 Mo4 O14 Mo1 75.6(3) . .
O11 Mo4 O14 Mo1 -74.7(8) . .
O12 Mo4 O14 Mo1 177.3(2) . .
O10 Mo4 O14 Mo1 -25.38(19) . .
O7 Mo4 O14 Mo1 -103.4(2) 3_667 .
Mo3 Mo4 O14 Mo1 -60.57(16) . .
O4W O5W O5WA O5WB -175(4) 2_656 .
